Abstract
Selfunfolding items provide a practical convenience, wherein ringlike frames are contorted into a state of equilibrium and subsequently pop up’ or deploy when perturbed from a folded structure. Can the same process be exploited at the molecular scale? At the limiting scale is a closed chain of single atoms, used here to investigate the limits of stability of such folded ring structures via full atomistic molecular dynamics. Carbyne is a onedimensional carbon allotrope composed of sphybridized carbon atoms. Here, we explore the stability of idealized carbyne loops as a function of chain length, curvature, and temperature, and delineate an effective phase diagram between folded and unfolded states. We find that while overall curvature is reduced, in addition to torsional and selfadhesive energy barriers, a local increase in curvature results in the largest impedance to unfolding.
Keywords:
Carbyne; Molecular dynamics; Unfolding; Adhesion; Torsion; Curvature; StabilityBackground
A clever trick by product designers is selfunfolding structures such as collapsible laundry hampers and popup’ tents. These ingenious designs involve a continuous ring structure that unfolds’ to a larger configuration. Similar mechanisms have been proposed for systems ranging from stretchable electronics [1] to polymer membranes [2,3] and hollow shell structures [4]. Here, we focus on the smallest possible unfolding system  a closed chain of carbon atoms  to investigate the limits of stability at the atomistic scale. Insights from such structures can then be applied to more complex macromolecular systems, such as responsive polymer [5,6] or proteinbased materials [710].
A simple molecular system capable of folding into a simple ring structure while maintaining atomistic fidelity and behavior is desired. As such, a model system is constructed using carbyne  a onedimensional carbon allotrope consisting of either a cumulative doublebond structure (cumulene) or alternating single and triple bonds (polyyne) [11,12]; the polyyne structure is depicted in Figure 1a. This 1D carbon structure has caused recent interest due to its novel electron transport and the prospect of being components in atomistic scale circuits [13,14], as well as recent synthesis of long chains [1519]. Previous firstprinciple and molecular dynamics (MD)based studies [2023] have characterized molecular mechanics (e.g., zero or nearzero temperatures) properties of isolated carbyne chains (e.g., in a vacuum). Considered here is a system of isolated closedloop carbyne (Figure 1b) to explore the stability of a folded threeloop geometry (Figure 1c).
Figure 1. Threeloop carbyne model and simulation. (a) Molecular structure of carbyne, a onedimensional carbon allotrope composed of sphybridized carbon atoms, consisting of alternating singletriple bonds. While chains of carbyne can be experimentally synthesized, they typically require heavy endgroups for stability [12,19]. (b) A theoretical carbyne loop’, circumventing the need for stabilizing endgroups by bonding the carbyne chain to itself. (c) Example molecular model of a folded carbyne loop in a stable threering configuration, with imposed overcurvature of three [68], similar to selfunfolding laundry hampers.
In simplest terms, additional elastic strain energy due to curvature triggers unfolding from the threeloop configuration. However, to completely unfold from an initial coiled state at the molecular scale, both torsional and selfadhesive energetic barriers must be overcome, resulting in a range of stable conditions, depending on initial curvature (κ) and temperature (T). In terms of coiled, looped, or otherwise convoluted geometries (such as knotted molecular structures [24,25]), a monoatomistic linear structure provides the simplest and most fundamental platform to explore stability and unfolding. Other systems, such as convoluted protein structures or DNA, would be more complex to analyze (due to kinetic hindrance of sidechain interactions, for example), but similar looped structures exist [2628] and are also dictated by a balance of thermal and mechanical contributions [2931].
While linear carbon chains have been experimentally attained, such a closed carbyne has yet to be synthesized. However, recent developments of carbon materials such as annulenes [3234] and extended porphyrins [35] suggest that carbon may allow such atomistic control’ and design of such molecular structures. Similar folded/looped atomistic structures include molecular knots [36,37], foldamers [38,39], and cyclic heterostructures [3942]. The use of homogeneous carbon eliminates the effects of more complex structures (such as torsional rigidity or steric interactions). However, while carbyne is used here as an idealized model system, the general behavior can serve as an analog to such systems and reflect the dynamics at a molecular scale.
Methods
Full atomistic simulations are implemented using classical MD, utilizing the firstprinciplebased ReaxFF potential [43,44], known to provide an accurate account of the chemical/mechanical behavior of carbon nanostructures [21,4549]. Due to a bond orderbased formulation, ReaxFF can reflect the bond hybridization of the polyyne structure of carbyne, as well as the effect of other valence terms (angle and torsion), without explicit parameterization [45]. It is noted that at such a scale, electron behavior may play a critical role. For example, a previous study demonstrated that in linear carbon chains, a local perturbation through the displacement of a single atom creates atomic force and charge density Friedellike oscillations [50]. Other electrondependent effects may include JahnTeller distortions [51] or Möbius topologies [52,53]. While such complex behavior is incapable of being replicated by MD potentials, it is deemed sufficient for the current scope of length and temperature effects on unfolding. A time step is chosen to be on the order of a fraction of femtoseconds (0.1 × 10^{15} s) to ensure the stability and reflect the high vibrational frequency of the acetylene groups of carbyne. All simulations are subject to a canonical (NVT) ensemble, with varying prescribed temperature (10 to 800 K), performed using the massively paralyzed modeling code LAMMPS (http://lammps.sandia.gov/ webcite) [54].
As carbyne has been stated to take either a cumulene (=C = C=) or a polyyne form (C ≡ C), small test structures (rings with n = 20 and n = 36) were minimized using ReaxFF to check the relative energetic stability of each structure (Figure 2). Cumulene has been reported to undergo a Peierls transition [55] into a polyyne form; our simulations confirm this instability, showing an energy difference in the order of 6.7 to 8.6 kcal mol^{1} atom^{1} in favor of the looped polyyne, in agreement with previous studies [55,56]. Moreover, beyond minimization, when nominal temperature was added to the ring structures, the cumulene rings transitioned to a triplesingle bond pattern, potentially due to the strain associated with the imposed curvature, which can facilitate the transition [57]. As the focus here is variation in temperature, only the polyyne configuration is stable throughout the range of temperatures used. Thus, all carbyne ring structures considered are reflective of polyyne structures. Initial threeloop systems are constructed with 54, 72, 90, 108, 126, 144, 162, and 180 carbon atoms, with associated ideal radii of approximately 4 to 13 Å. The threeloop fold pattern imposed is meant to maintain a nearconstant curvature across the total molecular length.
Figure 2. Relative molecular stability. Carbyne rings have been proposed as a transitional form of carbon during the synthesis of fullerenes [6063]. Other intermediate forms occurring with chain selfadhesion may form (e.g., socalled bow tie structures). To assess the stability of the rings during folding/threeloop configuration, the atomistic energy of cumulene rings and example intermediate’ structures was assessed with n = 20 (top, blue) and n = 36 (bottom, red) carbon atoms. We see that, aside from the fullerenes, the closedloop ring polyyne carbyne structures are more energetically favorable (lower energy) than the intermediates depicted, suggesting a relative stability for the equilibrium simulations undertaken.
In terms of the ring structure, while linear carbyne chains have been shown to be stable [19,58], imposing a closedloop geometry may be energetically unfavorable. To directly assess the stability of looped carbyne here, a linear chain was equilibrated to determine the difference in atomistic energy in comparison with the 54atom looped structure, resulting in a nominal difference of 0.02 eV atom^{1} and suggesting structural stability. For comparison, the energy difference between flat graphene and a fullerene is in the order of 0.2 eV atom^{1}[59], while the cohesive energy of carbyne has been found to be in the order of 6.99 [56] to 8.19 eV atom^{1}[50], in close agreement with the value of 7.4 eV atom^{1} calculated here at a finite temperature of 300 K.
We also wish to assess the stability in comparison with other noncarbyne molecular configurations. Empirically, similar ringlike structures with as few as 20 carbon atoms have been observed in the synthesis of fullerenes [60], as well as many intermediate bonded chain forms (e.g., socalled bow tie structures or cycloadducts) [6063]. To explore whether such intermediate forms may be energetically favorable, simple trial structures were equilibrated to assess the potential energy (also depicted in Figure 2), indicating that the looped/ring structure is more favorable than other intermediate forms. As depicted in Figure 2, the most energetically favorable structures are the fullerenes, with rings more favorable than that of the intermediate’ structures (in agreement with previous studies [61]; absolute relative energy differences would be dependent on the MD potential used). Increasing the bending energy (through folding) could increase the energy such that a transition may occur. That being said, the modeled structure not being the most energetically favorable does not imply that it cannot exist. Such an argument would indicate that fullerenes themselves should not exist, yet C_{20} fullerenes, bowls, and rings have been observed [60]. Less favorable intermediate structures are proposed pathways to fullerene synthesis [62,63] and can exhibit interesting properties or result in the synthesis of unique structures [64]. The focus here only involves the stability of a presumed folded structure.
The looped structures are equilibrated at a nominal temperature (10 K) and then subjected to temperature increase to a target temperature (with a rate of approximately 0.001 K fs^{1}) over 10 ps. As the molecular structures are isolated in a vacuum, the use of temperature as a variable is a direct measure of the kinetic energy of the atoms, independent of any insulating or damping effects an explicit solvent may contribute. Once the target temperature is reached, constant temperature is maintained, and the system is allowed to freely evolve for up to 0.1 ns to assess the stability of the configuration (test trials up to 5.0 ns were also ran to ensure equilibrium; in all cases, if unfolding was initiated, it occurred at a timescale less than 0.1 ns). The critical temperature of unfolding is then determined for each structure. Since the process is stochastic across the chain and the temperature is an ensemble average, the designated unfolding temperature only approximates the magnitude of energy required to trigger unfolding, and thus a range of critical temperatures emerges for the structures across multiple simulations. While the temperature variation was used to induce unfolding, of note is that the carbyne chains do not begin to disassociate until temperatures exceed approximately 3,500 K regardless of size (and a loss of any definitive curvature), defining an accessible temperature range for the ring structures.
Results and discussion
Root mean square deviation
Example snapshots of an unfolding loop are given in Figure 3, along with the associated root mean square deviation (RMSD) plot. The RMSD is defined as the spatial difference between two molecular structures:
where N denotes the number of atoms, r(t) denotes the position of each atom in the structure at time t, and r_{0} denotes the positions for the initial threeloop structure. A plateau of RMSD values indicates a locally stable structure and relative equilibrium. Due to the drastic structural transition between folded and unfolded states, RMSD can be used as a consistent metric to assess the stability of the global conformation [65,66]. The results indicate that unfolding occurs on a fast timescale on the order of tens of picoseconds once initiated. For comparison, such timescales have been observed on local/partial unfolding events of larger protein structures [66,67].
Figure 3. Simulation snapshots and root mean square displacement (or rmsd; see Equation 1) trajectories. Structures for n = 144 during low and hightemperature simulations. For low temperature (300 K, bottom), the folded threeloop structure remains stable and is an equilibrated state (indicated by the relatively constant RMSD). Increasing the temperature (750 K, top) induces unfolding, after which the unfolded structure equilibrates (larger variation in RMSD due to the oscillations induced by the momentum of unfolding).
Adhesion and torsional barriers
A recent macroscale investigation has determined that the way these rings behave depends on a single characteristic known as overcurvature [68] or how much more curved the threeloop configuration is than a flat circle of the same circumference. Here, each structure has the same initial overcurvature (equal to three). However, at the molecular scale, where temperature and selfadhesion effects are on the same energetic scale as strain energy, the relationship between curvature and stability is more complex. Indeed, due to the imposed overcurvature of the threeloop conformation, it could be anticipated that a relaxation of bending strain energy results in the necessary energy to unfold, assuming that the energy is sufficient to overcome the energy barrier due to adhesion and/or torsion (a full twist/rotation is necessary to unfold a looped chain).
Beyond the RMSD calculation, we track the associated potential energy of the carbyne system at a given temperature as it either remains stable (and in a threeloop configuration) or unfolds. Representative results are plotted in Figure 4. The given example indicates an energy barrier in the order of 200 kcal mol^{1} (for n = 126 and an unfolding temperature of 575 K). For all systems (54 to 180 atoms), the energy barriers were approximately 40 kcal mol^{1} (n = 54) to 400 kcal mol^{1} (n = 180), indicating a clear length dependence on the unfolding energy. To explore the magnitude of the absolute energy barrier due to torsion and adhesion, small simulations to explicitly quantify the energy of each contribution were undertaken independently (Figure 5).
Figure 4. Representative potential energy evolution for various temperatures (T = 100, 300, and 575 K) for n = 126. Initial heating phase (10 ps) increases energy due to temperature until either the structure remains in a folded, stable equilibrium (100, 300 K) or unfolding is triggered (575 K). Unfolding at the critical temperature is characterized by a drop in energy due to the release of bending strain energy and global increase in curvature. Here, the critical unfolding energy barrier is approximately 217 kcal mol^{1}.
Figure 5. Determining torsional and selfadhesion energy barriers. (a) Torsion: A simple fiveatom carbyne system with an imposed curvature (κ = 0.016 to 0.395 Å^{1}, inset κ = 0.2 Å^{1}) is subject to incremental twist while tracking the potential energy. The cyclical energy change due to a 180° twist increases with initial curvature as shown, defining the energy barrier (indicated by arrows) to untwist a carbyne chain in the looped configuration. (b) Adhesion: Three short sixatom carbyne chains (to reflect a threeloop adhesion case) were brought into close proximity over time to determine the interchain adhesion energy barrier, defined as the depth of the potential energy well (indicated by arrows).
For torsion, involving a complete rotation of the carbyne chain about itself, the associated energy barrier would be a function of the initial curvature. A simple fiveatom chain was constructed with a set of 14 initial curvatures ranging from 0.016 to 0.395 Å^{1} and subjected to incremental twist while tracking the potential energy (representative plots are given in Figure 5a). During the simulation, one terminal atom is fixed, along with the secondtothelast atom at the opposite end, while the adjacent terminal atom is then rotated about an axis of rotation and constant curvature maintained. The maximum energy barrier was calculated to be approximately 10 kcal mol^{1}, exhibited at large curvatures (>0.1 Å^{1}). A recent study quantified the torsional stiffness of carbyne, albeit using ab initio methods, a straight chain configuration, and the rotation of endgroups [56]. The reported energy barrier due to torsion ranged from approximately 0.2 to 0.6 eV, or 5 to 14 kcal mol^{1}. While the simulation approach and boundary conditions were different, the energy barrier determined here (approximately 10 kcal mol^{1}) is in the same order of magnitude and in a relatively good agreement. For adhesion, three carbyne chains were brought into contact and incrementally separated to determine the interchain adhesion energy (Figure 5b) of approximately 0.5 kcal mol^{1} atom^{1}. For the worst case scenario (the longest chain of 180 carbons resulting in three adhered 60 carbon rings plus the highest recorded torsional barrier), we calculate a maximum energy barrier of approximately 40 kcal mol^{1}  smaller than all but the minimum (n = 54) required energy increase indicated by the unfolding structures (also note that n = 54 unfolds with nominal kinetic energy required, at approximately T ≈ 10 K, representing the smallest possible stable threeloop structure). This indicates an additional contribution that must be overcome to induce unfolding, and we hence turn to the analysis of curvature.
Global and local curvature analysis
First, we assess the evolution of curvature between stable and unfolding structures through the equation [69]
where the derivatives with respect to the to the chain length, ŝ = 0 to L, and can be solved numerically through the coordinates of the atoms (Figure 6a,b). Representative results are depicted in Figure 6c, indicating the average radius of curvature
Figure 6. Curvature definition and global unfolding. (a) Defining local radius of curvature, r(ŝ), in the carbyne loop (ŝ = 0 to L), averaged to calculate the global radius of curvature and κ. (b) Schematic of coordinates used for the numerical solution to Equation 2, where each point represents adjacent carbon atoms. (c) Averaging the local curvatures across the molecule (here, n = 72 and n = 144) and calculating the associated radius of curvature, stable loop configurations have little change in radius at low temperatures (dashed arrows), while unfolding induced by high temperature results in a global increase in radius with respect to time (solid arrows) as anticipated (by definition, the unfolded structure will have a lower curvature).
To confirm, the local curvature is plotted as a function of time across the length of the carbyne molecule (Figure 7). Due to thermal fluctuations, the unfolding trajectory is highly stochastic, and the curvature plots are representative only. Both n = 72 and n = 144 are plotted as examples and are the same trajectories as the average curvatures plotted in Figure 6. For n = 72, a relatively low temperature is required for a stable threeloop structure (T = 50 K). Curvature is approximately constant (κ ≈ 0.27 Å^{1}, for a radius of approximately 3.7 Å) with slight variation along the molecular length due to temperatureinduced oscillations. The two peaks’ (κ ≈ 0.3 to 0.04 Å^{1}) occur approximately at the crossover of the carbon chains (see Figure 1c), necessitating a slight increase in local curvature. At a higher temperature (T = 200 K), there is enough energy to initiate unfolding. While globally the average radius increases, local unfolding induces increases in curvature in adjacent sections of the loop. Large peaks in the local curvature exceed 0.5 Å^{1} before the structure relaxes’ to a homogeneous, unfolded state (κ ≈ 0.12 Å^{1}). While limited in length, these increases in local curvature considerably impede unfolding at a low temperature and enhance stability in spite of the relatively high bending energy of the looped structure. For n = 144, again, low temperature results in a stable threeloop structure but at a higher range than n = 72 (T = 300 K, depicted). The thermal fluctuations and longer molecular length result in less prominent peaks as the effect of the crossover of the carbon chains is decreased. At a stable temperature, the curvature is relatively constant throughout the simulation (κ ≈ 0.11 Å^{1}, for a radius of approximately 9.0 Å). Increasing the temperature to induce unfolding again results in local increases in curvature to isolated sections of the molecule (exceeding 0.3 Å^{1}) while the average curvature decreases. Again, it is stressed that the peaks depicted in Figure 7 are stochastic and should be considered as representative only. However, all unfolded systems demonstrated significant increases in local curvature.
Figure 7. Local curvature, κ(ŝ,t). (a) Curvature across molecule for n = 72 at a stable low temperature (50 K). The curvature across the molecule is approximately constant (with thermal fluctuations); average, approximately 0.27 Å^{1}. (b) At a higher temperature (T = 200 K), the structure is unstable and undergoes unfolding. Unfolding induces localized increases in curvature resulting in large peaks (к → 0.5 Å^{1}) for sections of the molecule length. Once sufficient unfolding occurs, the structure approaches a homogeneous, unfolded state (κ ≈ 0.12 Å^{1}). (c) Curvature across molecule for n = 144 at a stable low temperature (300 K). Again, the curvature across the molecule is approximately constant; average, approximately 0.11 Å^{1}. (d) At a higher temperature (T = 725 K), the longer structure is unstable and undergoes unfolding. Again, unfolding induces localized increases in curvature resulting in large peaks (к → 0.3 Å^{1}) for sections of the molecule length. Once sufficient unfolding occurs, the structure approaches a homogeneous, unfolded state (κ ≈ 0.06 Å^{1}).
Critical unfolding temperatures
While the specific increases in curvature are nondeterministic, a simple model can be formulated to determine the critical unfolding temperature. To theoretically explore the stability of the folded carbon (or carbyne) loops, first the stored bending strain energy, U_{b}, in the system is defined, where [70]
where к denotes the initial imposed curvature of the carbyne chain of length L. During unfolding, it is assumed that there is a decrease in bending energy over portion of the length, αL, where α < 1.0, due to a decrease in curvature from к to βк, where β < 1.0. Thus, the amassed change in energy due this unfolding across the molecular length can be formulated as
Comparing to Equation 3, the change in energy due to local unfolding is a fraction of the total bending energy, as must be the case. The term α(1  β^{2}) < 1 by definition, where α captures the length of the chain unfolding and β is the decrease in curvature. In consideration of the simulation results, this is a stochastic term which cannot be calculated. We note that, due to thermal fluctuations, the curvature profile of the rings are constantly changing; calculating the bending strain energy for a particular case may result in a more accurate description for a single instance. Thus, we consider limiting cases only. The maximal case can be determined considering the upper bound of α = 1, wherein the entire loop may unfurl, and the minimum β. In the threeloop configuration, κ = 6π/L, while completely unfolded, κ = 2π/L, such that, for this particular structure, the lower bound of β is 1/3. With these two assumptions,
Moreover, noting again that κ = 6π/L,
Note that here D represents the effective bending stiffness. We also presume that carbyne behaves as a flexible molecular chain with a temperaturedependent flexibility and finite rigidity at zero temperature. A common property of molecular chains in polymer science is the persistence length, P, defined as the characteristic length over which direction can be correlated [71], related to both temperature (T) and bending rigidity (D). For flexible molecules, the persistence length can be approximated as P = D/k_{B}T, where k_{B} is the Boltzmann constant [72]. In a similar manner, persistence length is formulated here as a proxy for rigidity, assuming some finite persistence independent of temperature. As a consequence, the bending stiffness, D, can be directly represented as a function of temperature:
where P_{0} is considered the temperatureindependent persistence length. In effect, the apparent bending rigidity increases with temperature, also supported by previous theoretical results; a recent ab initio (temperaturefree) investigation reports the bending stiffness to be in the order of 5.3(10^{2}) nNnm^{2}[23], while a finite temperature (300 K) molecular dynamics study reports a stiffness of approximately 13 to 20(10^{2}) nNnm^{2}[21]. Here, D_{0} is the rigidity at zero temperature (as carbyne is not ideally flexible) and thus is approximated as 5.3(10^{2}) nNnm^{2}.
At the critical condition for unfolding, the gained strain energy (Equation 4) must be sufficient to overcome a local energy barrier, Ω, where Ω is a combination of adhesion energy and required strain energy to unfold (e.g., local increase in curvature as depicted in Figure 7 and torsional and adhesion contributions) such that ΔU_{b} = Ω. Substituting (4) into (3c) and rearranging to solve for temperature results in
Using Equation 6 with the simulation results, the approximate unfolding temperature, T_{unfolding}, can be predicted. The key assumption is that the unfolding process does not imply a constant decrease in energy (i.e., release of bending strain energy), and thus some energetic input, Ω, is required to allow deviation from the highenergy folded or looped state, which can be considered a temperaturedependent state of quasiequilibrium. The maximum and minimum observed unfolding temperatures of each molecular length are plotted and fitted by linear regression (Figure 8). From the fitted parameters and assuming D_{0} ≅ 5.3(10^{2}) nNnm^{2}, both P_{0} and Ω can be calculated. From the temperature intercept (204 ± 142 K), P_{0} is estimated as 110 to 610 Å (best fit with P_{0} = 187 Å). Note that this is not considered the persistence length of carbyne but only a temperatureindependent contribution (such that carbyne will display finite persistence even at high temperatures) and thus a lower bound. As a comparison, the persistence length of DNA is similarly in the order of tens of nanometers [73,74]. Using the best fit value of P_{0} and Equation 5, the increase in stiffness for finite temperatures can be calculated. A temperature of 300 K results in a bending stiffness of 13.0 nNnm^{2}, in good agreement with previous computational results [21].
Figure 8. Critical unfolding temperature (T_{unfolding}) versus molecule length. Due to the stochastic nature of unfolding, simulation results indicate a range of possible unfolding temperatures for each length of carbyne model. The maximum and minimum of each length are plotted. For example, for n = 126 (L ≅ 170 Å), both unfolding and stable structures were observed at temperatures from 575 to 650 K (points plotted), but all simulations above 650 K unfolded, and all below 575 K remained stable. The results were fitted with a linear regression (red line), resulting in a temperature intercept of 204 ± 142 K and a slope of 4.2 ± 0.85 K Å^{1} (with an associated R^{2} value of 0.889). The results can be associated with Equation 6. The regression can be used to delineate the folded (stable) and unfolded (unstable) states in an effective phase diagram. The 90% confidence intervals are also plotted, encapsulating all observed data points.
Using the fitted slope of 4.2 ± 0.85 K Å^{1}, the energy barrier to unfolding, Ω, is determined to be approximately 98 to 366 kcal mol^{1} (best fit with Ω = 139 kcal mol^{1}), which agrees well with the magnitude of measured energy barriers (40 to 400 kcal mol^{1}). This range may be seemingly large as the energy of cohesion for the chains is in the order of 7 eV or approximately 160 kcal mol^{1}; one may expect the chains to break before unfolding. However, the barrier is due to the bending strain energy required, which, by definition, requires the involvement of numerous atoms (rather than a single cleavage site [75], for example). In consideration of the relatively large flexural rigidity of carbyne, such bending energy barriers can be quite significant. If we consider the change in curvature for n = 72, from approximately 0.27 Å^{1} to local peaks of 0.5 Å^{1}, then we can approximate the length that undergoes the local increase in curvature by equating the energy barrier, Ω, with the local bending strain energy. For n = 72 at 200 K (for a bending rigidity of D_{200K} = 10.4 nNnm^{2} by Equation 5), this results in local curvature increase in approximately 7.4 to 27.5 Å of the loop. This range of length is in good agreement with the size/span of the peaks depicted in Figure 8. Similarly, considering n = 144 at 725 K (for a bending rigidity of D_{725K} = 24.0 nNnm^{2}), with curvature increases from 0.11 Å^{1} to local peaks of 0.3 Å^{1}, results in local curvature increasing in approximately 7.2 Å to 27.2 Å to develop the determined energy barrier, again in good agreement with Figure 8, which indicated multiple (but short spanning) peaks across the molecular length. It is noted that there is an intrinsic relationship between the magnitude of local curvature and necessary length, i.e., a longer length can develop the equivalent energy barrier with a smaller curvature as U_{b} ∝ Lк^{2}.
Conclusions
The results confirm that, while global unfolding implies an overall reduction in curvature, continuity of the molecular loop results in local increases in curvature, resulting in a small yet finite energy barrier to surpass. For longer loops (with less stored bending strain energy due to a decrease in curvature), a higher temperature (e.g., kinetic energy) is required to induce unfolding. In contrast, short loops (with high bending energies) unfold at relatively low temperatures. Using carbyne as a platform, the potential for folding can serve to extend the accessible design space of such materials. It is noted that the heterogeneous/local curvature as depicted in the snapshots in Figure 3, as well as plotted in Figure 7, was not explicitly considered in terms of energy contribution. Rather, the limiting cases  the curvature of the threeloop structure and the curvature of an unfolded ring  were used to estimate the necessary energy. Here, all structures begin in an ideal configuration, and the deviations from the ideal curvatures are due to thermal fluctuations; the thermal energy (essentially molecular kinetic energy) must impose overcurvature to trigger the unfolding process. Since the heterogeneous curvatures are stochastic (the results plotted are only representative), temperature is used as a proxy to evaluate the necessary energy to unfold.
It behooves us to note that the looped carbyne structure modeled herein is not attainable experimentally and is intended as an ideal model platform to explore the unfolding phenomena. A similar idealized beadspringtype’ model could have been constructed but would be subject to the arbitrariness of parameterization. Carbyne provides a compromise  an ideal structure with physical, fundamental, and proven molecularscale parameterization/behavior through the ReaxFF potential. It is the simplest case from a molecular perspective (a nonreactive homogeneous chain, no solvent, etc.) and is necessary to isolate and observe the thermal contribution to unfolding as well as the local curvature effect. Indeed, understanding the stability and mechanics of folded carbyne loops can be of use in modifying transport properties or triggering mechanisms in active molecular systems.
Finally, understanding the mechanical principles of such geometries will help not only in dissecting existing looped systems but also in designing and constructing commercially useful selfassembling nanostructures. For example, the local curvature increase may be isolated in a particular, flexible molecular hinge’ or activated by an enzyme in biological systems. When one thinks of folding/unfolding at the molecular scale, DNA and similarly protein structures are likely to come to mind. In terms of insights to such structures, the governing folding/unfolding phenomenon is quite different from carbyne loops. However, there are insights even from this simple system; DNA can exhibit looped configurations, which can serve to suppress the formation of gene products, or facilitate compaction of DNA as a whole [2631,76,77]. The size of the loops also affects the mechanical stability [2628] and has been analyzed via elastic assumptions [29] and thermodynamic cost [30]. Similar to the carbyne system here, larger loops are shown to be more stable. The observation that local curvature undergoes an increase may shed light into the attainment of such structures. Indeed, for small DNA looped structures to be stable, extensive local curvature is required (which can be potentially controlled by sequence; see [77] and references therein). While at a different scale, clearly there is an interplay between curvature, local flexibility, and temperature similar to that of the structures observed here. There are no direct insights from carbyne to macromolecules such as DNA, just as the general study of overcurvature in collapsible laundry baskets was not applied at the molecular scale here. But there are indeed potential indirect corollaries.
While carbon chains have been primarily studied as extensions from graphene [78] or carbon nanotubes [79,80], isolated carbynes and related structures may inspire an even smaller generation of nanomaterials, with increased functionality due to their intrinsic flexibility and ability to attain exotic topologies. Development of looped systems may lead to novel devices that unfold’ per design with some external event  a potential novel nanoscale trigger  motivated by commercial popup tents and collapsible laundry hampers.
Competing interests
The author declares no competing interests.
Acknowledgements
S.W.C. acknowledges the generous support from NEU's CEE Department. The calculations and the analysis were carried out using a parallel LINUX cluster at NEU's Laboratory for Nanotechnology In Civil Engineering (NICE).
References

Sun YG, Choi WM, Jiang HQ, Huang YGY, Rogers JA: Controlled buckling of semiconductor nanoribbons for stretchable electronics.
Nat Nanotechnol 2006, 1:201207. PubMed Abstract  Publisher Full Text

Klein Y, Efrati E, Sharon E: Shaping of elastic sheets by prescription of nonEuclidean metrics.
Science 2007, 315:11161120. PubMed Abstract  Publisher Full Text

Kim J, Hanna JA, Byun M, Santangelo CD, Hayward RC: Designing responsive buckled surfaces by halftone gel lithography.
Science 2012, 335:12011205. PubMed Abstract  Publisher Full Text

Shim J, Perdigou C, Chen ER, Bertoldi K, Reis PM: Bucklinginduced encapsulation of structured elastic shells under pressure.
Proc Natl Acad Sci USA 2012, 109:59785983. PubMed Abstract  Publisher Full Text  PubMed Central Full Text

Guan JJ, He HY, Lee LJ, Hansford DJ: Fabrication of particulate reservoircontaining, capsulelike, and selffolding polymer microstructures for drug delivery.
Small 2007, 3:412418. PubMed Abstract  Publisher Full Text

Ionov L: Soft microorigami: selffolding polymer films.
Soft Matter 2011, 7:67866791. Publisher Full Text

Stepanskiy LG: Sonicationinduced unfolding proteins.
J Theor Biol 2012, 298:7781. PubMed Abstract  Publisher Full Text

Neidigh JW, Fesinmeyer RM, Andersen NH: Designing a 20residue protein.
Nat Struct Biol 2002, 9:425430. PubMed Abstract  Publisher Full Text

Sulkowska JI, Noel JK, Onuchic JN: Energy landscape of knotted protein folding.
Proc Natl Acad Sci USA 2012, 109:1778317788. PubMed Abstract  Publisher Full Text  PubMed Central Full Text

Dean FB, Stasiak A, Koller T, Cozzarelli NR: Duplex DNA knots produced by Escherichia coli topoisomerase I  structure and requirements for formation.
J Biol Chem 1985, 260:49754983. PubMed Abstract  Publisher Full Text

Kavan L, Kastner J: Carbyne forms of carbon: continuation of the story.
Carbon 1994, 32:15331536. Publisher Full Text

Chalifoux WA, Ferguson MJ, McDonald R, Melin F, Echegoyen L, Tykwinski RR: Adamantylendcapped polyynes.
J Phys Org Chem 2012, 25:6976. Publisher Full Text

Lin ZZ, Ning XJ: Controlling the electronic properties of monatomic carbon chains.
EplEurophys Lett 2011, 95:47012. Publisher Full Text

Khoo KH, Neaton JB, Son YW, Cohen ML, Louie SG: Negative differential resistance in carbon atomic wirecarbon nanotube junctions.
Nano Lett 2008, 8:29002905. PubMed Abstract  Publisher Full Text

Tykwinski RR, Chalifoux W, Eisler S, Lucotti A, Tommasini M, Fazzi D, Del Zoppo M, Zerbi G: Toward carbyne: synthesis and stability of really long polyynes.
Pure Appl Chem 2010, 82:891904. Publisher Full Text

Gibtner T, Hampel F, Gisselbrecht JP, Hirsch A: Endcap stabilized oligoynes: model compounds for the linear sp carbon allotrope carbyne.
ChemEur J 2002, 8:408432. Publisher Full Text

Cataldo F: A method for synthesizing polyynes in solution.
Carbon 2005, 43:27922800. Publisher Full Text

Eisler S, Slepkov AD, Elliott E, Luu T, McDonald R, Hegmann FA, Tykwinski RR: Polyynes as a model for carbyne: synthesis, physical properties, and nonlinear optical response.
J Am Chem Soc 2005, 127:26662676. PubMed Abstract  Publisher Full Text

Chalifoux WA, Tykwinski RR: Synthesis of polyynes to model the spcarbon allotrope carbyne.
Nat Chem 2010, 2:967971. PubMed Abstract  Publisher Full Text

Itzhaki L, Altus E, Basch H, Hoz S: Harder than diamond: determining the crosssectional area and Young's modulus of molecular rods.
Angew Chem Int Edit 2005, 44:74327435. Publisher Full Text

Nair AK, Cranford SW, Buehler MJ: The minimal nanowire: mechanical properties of carbyne.
EplEurophys Lett 2011, 95:16002. Publisher Full Text

Hu YH: Bending effect of sphybridized carbon (carbyne) chains on their structures and properties.
The Journal of Physical Chemistry C 2011, 115:18431850. Publisher Full Text

Castelli IE, Salvestrini P, Manini N: Mechanical properties of carbynes investigated by ab initio totalenergy calculations.

Dobrowolski JC, Mazurek AP: Model carbyne knots vs ideal knots.
J Chem Inf Comp Sci 2003, 43:861869. Publisher Full Text

Deng WY, Qiu WY: Helical chirality in model mirrorimaged carbyne trefoil knots.
J Mol Struct 2008, 875:515519. Publisher Full Text

Becker NA, Kahn JD, Maher LJ: Bacterial repression loops require enhanced DNA flexibility.
J Mol Biol 2005, 349:716730. PubMed Abstract  Publisher Full Text

Yuann JMP, Tseng WH, Lin HY, Hou MH: The effects of loop size on Sac7dhairpin DNA interactions.
BbaProteins Proteom 2012, 1824:10091015. Publisher Full Text

Vafabakhsh R, Ha T: Extreme bendability of DNA less than 100 base pairs long revealed by singlemolecule cyclization.
Science 2012, 337:10971101. PubMed Abstract  Publisher Full Text  PubMed Central Full Text

Cherstvy AG: Looping charged elastic rods: applications to proteininduced DNA loop formation.
Eur Biophys J Biophy 2011, 40:6980. Publisher Full Text

Levene SD, Giovan SM, Hanke A, Shoura MJ: The thermodynamics of DNA loop formation, from J to Z.
Biochem Soc T 2013, 41:513518. Publisher Full Text

Olson WK, Grosner MA, Czapla L, Swigon D: Structural insights into the role of architectural proteins in DNA looping deduced from computer simulations.
Biochem Soc T 2013, 41:559564. Publisher Full Text

Spitler EL, Johnson CA, Haley MM: Renaissance of annulene chemistry.
Chem Rev 2006, 106:53445386. PubMed Abstract  Publisher Full Text

Stevenson CD: Annulenylenes, annulynes, and annulenes.
Accounts Chem Res 2007, 40:703711. Publisher Full Text

Castro C, Karney WL: Mechanisms and Mobius strips: understanding dynamic processes in annulenes.
J Phys Org Chem 2012, 25:612619. Publisher Full Text

Saito S, Osuka A: Expanded porphyrins: intriguing structures, electronic properties, and reactivities.
Angew Chem Int Edit 2011, 50:43424373. Publisher Full Text

Lukin O, Vogtle F: Knotting and threading of molecules: chemistry and chirality of molecular knots and their assemblies.
Angew Chem Int Edit 2005, 44:14561477. Publisher Full Text

Andrae D: Molecular knots, links, and fabrics: prediction of existence and suggestion of a synthetic route.
New J Chem 2006, 30:873882. Publisher Full Text

Ghosh K, Moore JS: Foldamer structuring by covalently bound macromolecules.
J Am Chem Soc 2011, 133:1965019652. PubMed Abstract  Publisher Full Text

Yamato K, Kline M, Gong B: Cavitycontaining, backbonerigidified foldamers and macrocycles.
Chem Commun 2012, 48:1214212158. Publisher Full Text

Fu HL, Liu Y, Zeng HQ: Shapepersistent Hbonded macrocyclic aromatic pentamers.
Chem Commun 2013, 49:41274144. Publisher Full Text

Sisco SW, Moore JS: Directional cyclooligomers via alkyne metathesis.
J Am Chem Soc 2012, 134:91149117. PubMed Abstract  Publisher Full Text

Hoger S: Shapepersistent phenyleneacetylene macrocycles: large ringslow yield?
Angew Chem Int Edit 2005, 44:38063808. Publisher Full Text

Chenoweth K, Van Duin ACT, Goddard WA: ReaxFF reactive force field for molecular dynamics simulations of hydrocarbon oxidation.
J Phys Chem A 2008, 112:10401053. PubMed Abstract  Publisher Full Text

Strachan A, Kober EM, Van Duin ACT, Oxgaard J, Goddard WA: Thermal decomposition of RDX from reactive molecular dynamics.
J Chem Phys 2005, 122:054502. Publisher Full Text

Van Duin ACT, Dasgupta S, Lorant F, Goddard WA: ReaxFF: a reactive force field for hydrocarbons.
J Phys Chem A 2001, 105:93969409. Publisher Full Text

Nielson KD, Van Duin ACT, Oxgaard J, Deng WQ, Goddard WA: Development of the ReaxFF reactive force field for describing transition metal catalyzed reactions, with application to the initial stages of the catalytic formation of carbon nanotubes.
J Phys Chem A 2005, 109:493499. PubMed Abstract  Publisher Full Text

Chen N, Lusk MT, VanDuin ACT, Goddard WA: Mechanical properties of connected carbon nanorings via molecular dynamics simulation.

Buehler MJ: Mesoscale modeling of mechanics of carbon nanotubes: selfassembly, selffolding, and fracture.
J Mater Res 2006, 21:28552869. Publisher Full Text

Cranford SW, Buehler MJ: Mechanical properties of graphyne.
Carbon 2011, 49:41114121. Publisher Full Text

Cahangirov S, Topsakal M, Ciraci S: Longrange interactions in carbon atomic chains.

Kato T, Yoshizawa K, Yamabe T: Vibronic coupling and JahnTeller effects in negatively charged [30]annulene.
Chem Phys 1999, 247:375386. Publisher Full Text

Rzepa HS: Mobius aromaticity and delocalization.
Chem Rev 2005, 105:36973715. PubMed Abstract  Publisher Full Text

Herges R: Topology in chemistry: designing Mobius molecules.
Chem Rev 2006, 106:48204842. PubMed Abstract  Publisher Full Text

Plimpton S: Fast parallel algorithms for shortrange moleculardynamics.
J Comput Phys 1995, 117:119. Publisher Full Text

Kertesz M, Koller J, Azman A: Ab initio HartreeFock crystal orbital studies. 2. Energybands of an infinite carbon chain.
J Chem Phys 1978, 68:27792782. Publisher Full Text

Liu M, Artyukhov VI, Lee H, Xu F, Yakobson BI: Carbyne from first principles: chain of C atoms, a nanorod or a nanorope.
Acs Nano 2013.
doi:10.1021/nn404177r

Artyukhov VI, Liu M, Yakobson BI: Mechanically induced metalinsulator transition in carbyne.
arXiv:13027250.

Lin ZZ, Yu WF, Wang Y, Ning XJ: Predicting the stability of nanodevices.
EplEurophys Lett 2011, 94:40002. Publisher Full Text

Chuvilin A, Kaiser U, Bichoutskaia E, Besley NA, Khlobystov AN: Direct transformation of graphene to fullerene.
Nat Chem 2010, 2:450453. PubMed Abstract  Publisher Full Text

Prinzbach H, Weller A, Landenberger P, Wahl F, Worth J, Scott LT, Gelmont M, Olevano D, Von Issendorff B: Gasphase production and photoelectron spectroscopy of the smallest fullerene, C20.
Nature 2000, 407:6063. PubMed Abstract  Publisher Full Text

Allison C, Beran KA: Energetic analysis of 24 C20 isomers.
J Mol StrucTheochem 2004, 680:5963. Publisher Full Text

Goroff NS: Mechanism of fullerene formation.
Accounts Chem Res 1996, 29:7783. Publisher Full Text

Strout DL, Scuseria GE: A cycloaddition model for fullerene formation.
J Phys ChemUs 1996, 100:64926498. Publisher Full Text

Kawasumi K, Zhang Q, Segawa Y, Scott LT, Itami K: A grossly warped nanographene and the consequences of multiple oddmemberedring defects.
Nat Chem 2013, 5:739744. PubMed Abstract  Publisher Full Text

Grossfield A, Zuckerman DM: Quantifying uncertainty and sampling quality in biomolecular simulations.

Lazaridis T, Karplus M: “New view” of protein folding reconciled with the old through multiple unfolding simulations.
Science 1997, 278:19281931. PubMed Abstract  Publisher Full Text

Thielges MC, Fayer MD: Protein dynamics studied with ultrafast twodimensional infrared vibrational echo spectroscopy.
Accounts Chem Res 2012, 45:18661874. Publisher Full Text

Mouthuy PO, Coulombier M, Pardoen T, Raskin JP, Jonas AM: Overcurvature describes the buckling and folding of rings from curved origami to foldable tents.
Nat Commun 2012, 3:1290. PubMed Abstract  Publisher Full Text  PubMed Central Full Text

Rutter JW: Geometry of Curves. Boca Raton: Chapman & Hall; 2000.

Landau LD, Lifshitz EM: Theory of Elasticity. 2nd English edn. Oxford: Pergamon Press; 1970.

Grosberg AIU, Khokhlov AR: Statistical Physics of Macromolecules. New York: AIP Press; 1994.

Yamakawa H: Modern Theory of Polymer Solutions. New York: Harper & Row; 1971.

Hagerman PJ: Flexibility of DNA.
Annu Rev Biophys Bio 1988, 17:265286. Publisher Full Text

Brinkers S, Dietrich HRC, De Groote FH, Young IT, Rieger B: The persistence length of double stranded DNA determined using dark field tethered particle motion.
J Chem Phys 2009, 130:215105. PubMed Abstract  Publisher Full Text

Moras G, Pastewka L, Walter M, Schnagl J, Gumbsch P, Moseler M: Progressive shortening of sphybridized carbon chains through oxygeninduced cleavage.
J Phys Chem C 2011, 115:2465324661. Publisher Full Text

Semsey S, Virnik K, Adhya S: A gamut of loops: meandering DNA.
Trends Biochem Sci 2005, 30:334341. PubMed Abstract  Publisher Full Text

Zhang Y, McEwen AE, Crothers DM, Levene SD: Statisticalmechanical theory of DNA looping.
Biophys J 2006, 90:19031912. PubMed Abstract  Publisher Full Text  PubMed Central Full Text

Castelli IE, Ferri N, Onida G, Manini N: Carbon sp chains in graphene nanoholes.
J PhysCondens Mat 2012, 24:104019. Publisher Full Text

Xu B, Lin JY, Lim SH, Feng YP: Structural and electronic properties of finite carbon chains encapsulated into carbon nanotubes.
J Phys Chem C 2009, 113:2131421318. Publisher Full Text

Zhao XL, Ando Y, Liu Y, Jinno M, Suzuki T: Carbon nanowire made of a long linear carbon chain inserted inside a multiwalled carbon nanotube.
Phys Rev Lett 2003, 90:187401. PubMed Abstract  Publisher Full Text